#------------------------------------------------------------------------------
#$Date: 2016-03-21 17:09:55 +0200 (Mon, 21 Mar 2016) $
#$Revision: 178771 $
#$URL: svn://www.crystallography.net/cod/cif/4/10/25/4102593.cif $
#------------------------------------------------------------------------------
#
# This file is available in the Crystallography Open Database (COD),
# http://www.crystallography.net/
#
# All data on this site have been placed in the public domain by the
# contributors.
#
data_4102593
loop_
_publ_author_name
'Peng Wang'
'Scott Forbes'
'Taras Kolodiazhnyi'
'Kosuke Kosuda'
'Yurij Mozharivskyj'
_publ_section_title
;
 Synthesis, Crystal and Electronic Structures of New Narrow-Band-Gap
 Semiconducting Antimonide Oxides RE3SbO3 and RE8Sb3-\dO8, with RE = La,
 Sm, Gd, and Ho
;
_journal_name_full               'Journal of the American Chemical Society'
_journal_page_first              8795
_journal_page_last               8803
_journal_paper_doi               10.1021/ja1027698
_journal_volume                  132
_journal_year                    2010
_chemical_formula_sum            'Ho8 O8 Sb3'
_chemical_formula_weight         1812.69
_chemical_name_systematic
; 
 ? 
;
_space_group_IT_number           12
_symmetry_cell_setting           monoclinic
_symmetry_space_group_name_Hall  '-C 2y'
_symmetry_space_group_name_H-M   'C 1 2/m 1'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 106.958(7)
_cell_angle_gamma                90.00
_cell_formula_units_Z            2
_cell_length_a                   13.1368(11)
_cell_length_b                   3.7609(2)
_cell_length_c                   14.8700(13)
_cell_measurement_reflns_used    20510
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      75.0
_cell_measurement_theta_min      7.3
_cell_volume                     702.73(10)
_computing_cell_refinement       X-Area
_computing_data_collection       X-Area
_computing_data_reduction        X-Red32
_computing_publication_material  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 1997)'
_computing_structure_solution    'SHELXS-97 (Sheldrick, 1990)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.994
_diffrn_measured_fraction_theta_max 0.994
_diffrn_measurement_device_type  'STOE IPDSII'
_diffrn_measurement_method       'omega scan'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0900
_diffrn_reflns_av_sigmaI/netI    0.0724
_diffrn_reflns_limit_h_max       22
_diffrn_reflns_limit_h_min       -22
_diffrn_reflns_limit_k_max       6
_diffrn_reflns_limit_k_min       -6
_diffrn_reflns_limit_l_max       25
_diffrn_reflns_limit_l_min       -25
_diffrn_reflns_number            10299
_diffrn_reflns_theta_full        37.20
_diffrn_reflns_theta_max         37.20
_diffrn_reflns_theta_min         3.65
_exptl_absorpt_coefficient_mu    50.125
_exptl_absorpt_correction_T_max  0.2546
_exptl_absorpt_correction_T_min  0.0674
_exptl_absorpt_correction_type   numerical
_exptl_absorpt_process_details   X-Red
_exptl_crystal_colour            Black
_exptl_crystal_density_diffrn    8.567
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       Plate
_exptl_crystal_F_000             1506
_exptl_crystal_size_max          0.028
_exptl_crystal_size_mid          0.025
_exptl_crystal_size_min          0.008
_refine_diff_density_max         4.309
_refine_diff_density_min         -4.141
_refine_diff_density_rms         0.719
_refine_ls_extinction_coef       0.00185(6)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc²λ³/sin(2θ)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.015
_refine_ls_matrix_type           full
_refine_ls_number_parameters     62
_refine_ls_number_reflns         2022
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.015
_refine_ls_R_factor_all          0.0737
_refine_ls_R_factor_gt           0.0410
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[σ²(Fo²)+(0.0241P)²+0.0000P] where P=(Fo²+2Fc²)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0660
_refine_ls_wR_factor_ref         0.0720
_reflns_number_gt                1458
_reflns_number_total             2022
_reflns_threshold_expression     >2sigma(I)
_cod_data_source_file            ja1027698_si_008.cif
_cod_data_source_block           c2m
_cod_original_cell_volume        702.73(9)
_cod_database_code               4102593
loop_
_symmetry_equiv_pos_as_xyz
'x, y, z'
'-x, y, -z'
'x+1/2, y+1/2, z'
'-x+1/2, y+1/2, -z'
'-x, -y, -z'
'x, -y, z'
'-x+1/2, -y+1/2, -z'
'x+1/2, -y+1/2, z'
loop_
_atom_site_label
_atom_site_type_symbol
_atom_site_fract_x
_atom_site_fract_y
_atom_site_fract_z
_atom_site_U_iso_or_equiv
_atom_site_adp_type
_atom_site_occupancy
_atom_site_symmetry_multiplicity
_atom_site_calc_flag
_atom_site_refinement_flags
Ho1 Ho 0.71926(4) 0.0000 0.08908(4) 0.00718(11) Uani 1 2 d S
Ho2 Ho 0.45628(4) 0.0000 0.16929(4) 0.01116(12) Uani 1 2 d S
Ho3 Ho 0.87741(4) 0.0000 0.34761(4) 0.00739(11) Uani 1 2 d S
Ho4 Ho 0.64347(4) 0.0000 0.43042(4) 0.00859(11) Uani 1 2 d S
Sb1 Sb 0.17137(6) 0.0000 0.26664(6) 0.01297(17) Uani 1 2 d S
Sb2 Sb 0.0000 0.0504(11) 0.0000 0.0123(10) Uani 0.475(4) 2 d SP
O1 O 0.4691(6) 0.0000 0.3688(9) 0.023(2) Uani 1 2 d S
O2 O 0.8826(7) 0.0000 0.2018(5) 0.0100(15) Uani 1 2 d S
O3 O 0.2960(6) 0.0000 0.0663(6) 0.0083(14) Uani 1 2 d S
O4 O 0.1649(6) 0.0000 0.5144(6) 0.0091(14) Uani 1 2 d S
loop_
_atom_type_symbol
_atom_type_description
_atom_type_scat_dispersion_real
_atom_type_scat_dispersion_imag
_atom_type_scat_source
O O 0.0106 0.0060 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Sb Sb -0.5866 1.5461 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
Ho Ho -0.2175 4.6783 'International Tables Vol C Tables 4.2.6.8 and 6.1.1.4'
loop_
_geom_angle_atom_site_label_1
_geom_angle_atom_site_label_2
_geom_angle_atom_site_label_3
_geom_angle
_geom_angle_site_symmetry_1
_geom_angle_site_symmetry_3
O3 Ho1 O3 116.9(4) 3 3_545
O3 Ho1 O3 75.6(2) 3 5_655
O3 Ho1 O3 75.6(2) 3_545 5_655
O3 Ho1 O2 75.0(2) 3 .
O3 Ho1 O2 75.0(2) 3_545 .
O3 Ho1 O2 122.0(3) 5_655 .
O3 Ho1 Sb2 140.08(18) 3 3_545
O3 Ho1 Sb2 83.41(18) 3_545 3_545
O3 Ho1 Sb2 77.32(17) 5_655 3_545
O2 Ho1 Sb2 144.88(10) . 3_545
O3 Ho1 Sb2 83.41(18) 3 7
O3 Ho1 Sb2 140.08(18) 3_545 7
O3 Ho1 Sb2 77.32(17) 5_655 7
O2 Ho1 Sb2 144.88(10) . 7
Sb2 Ho1 Sb2 62.30(12) 3_545 7
O3 Ho1 Sb1 81.2(2) 3 3
O3 Ho1 Sb1 141.0(2) 3_545 3
O3 Ho1 Sb1 143.29(8) 5_655 3
O2 Ho1 Sb1 77.43(17) . 3
Sb2 Ho1 Sb1 104.87(4) 3_545 3
Sb2 Ho1 Sb1 72.06(3) 7 3
O3 Ho1 Sb1 141.0(2) 3 3_545
O3 Ho1 Sb1 81.2(2) 3_545 3_545
O3 Ho1 Sb1 143.29(8) 5_655 3_545
O2 Ho1 Sb1 77.43(17) . 3_545
Sb2 Ho1 Sb1 72.06(3) 3_545 3_545
Sb2 Ho1 Sb1 104.87(4) 7 3_545
Sb1 Ho1 Sb1 66.151(19) 3 3_545
O3 Ho1 Sb2 144.42(18) 3 7_545
O3 Ho1 Sb2 78.42(18) 3_545 7_545
O3 Ho1 Sb2 78.11(15) 5_655 7_545
O2 Ho1 Sb2 140.20(9) . 7_545
Sb2 Ho1 Sb2 5.35(12) 3_545 7_545
Sb2 Ho1 Sb2 67.651(14) 7 7_545
Sb1 Ho1 Sb2 107.49(3) 3 7_545
Sb1 Ho1 Sb2 69.59(3) 3_545 7_545
O3 Ho1 Sb2 78.42(18) 3 3
O3 Ho1 Sb2 144.42(18) 3_545 3
O3 Ho1 Sb2 78.11(15) 5_655 3
O2 Ho1 Sb2 140.20(9) . 3
Sb2 Ho1 Sb2 67.651(14) 3_545 3
Sb2 Ho1 Sb2 5.35(12) 7 3
Sb1 Ho1 Sb2 69.59(3) 3 3
Sb1 Ho1 Sb2 107.49(3) 3_545 3
Sb2 Ho1 Sb2 73.00(11) 7_545 3
O3 Ho1 Ho1 97.1(2) 3 7_645
O3 Ho1 Ho1 38.3(2) 3_545 7_645
O3 Ho1 Ho1 37.27(9) 5_655 7_645
O2 Ho1 Ho1 100.21(17) . 7_645
Sb2 Ho1 Ho1 77.74(3) 3_545 7_645
Sb2 Ho1 Ho1 109.81(4) 7 7_645
Sb1 Ho1 Ho1 177.36(3) 3 7_645
Sb1 Ho1 Ho1 114.668(10) 3_545 7_645
Sb2 Ho1 Ho1 75.08(3) 7_545 7_645
Sb2 Ho1 Ho1 112.11(3) 3 7_645
O3 Ho1 Ho1 38.3(2) 3 7_655
O3 Ho1 Ho1 97.1(2) 3_545 7_655
O3 Ho1 Ho1 37.27(9) 5_655 7_655
O2 Ho1 Ho1 100.21(17) . 7_655
Sb2 Ho1 Ho1 109.81(4) 3_545 7_655
Sb2 Ho1 Ho1 77.74(3) 7 7_655
Sb1 Ho1 Ho1 114.668(10) 3 7_655
Sb1 Ho1 Ho1 177.36(3) 3_545 7_655
Sb2 Ho1 Ho1 112.11(3) 7_545 7_655
Sb2 Ho1 Ho1 75.08(3) 3 7_655
Ho1 Ho1 Ho1 64.393(19) 7_645 7_655
O3 Ho2 O2 76.4(2) . 3_445
O3 Ho2 O2 76.4(2) . 3_455
O2 Ho2 O2 114.9(4) 3_445 3_455
O3 Ho2 Sb2 79.0(2) . 3_545
O2 Ho2 Sb2 85.08(19) 3_445 3_545
O2 Ho2 Sb2 143.1(2) 3_455 3_545
O3 Ho2 Sb2 79.0(2) . 7
O2 Ho2 Sb2 143.1(2) 3_445 7
O2 Ho2 Sb2 85.08(19) 3_455 7
Sb2 Ho2 Sb2 63.35(13) 3_545 7
O3 Ho2 Sb1 144.20(7) . 3
O2 Ho2 Sb1 138.0(2) 3_445 3
O2 Ho2 Sb1 78.3(2) 3_455 3
Sb2 Ho2 Sb1 108.19(4) 3_545 3
Sb2 Ho2 Sb1 73.91(4) 7 3
O3 Ho2 Sb1 144.20(7) . 3_545
O2 Ho2 Sb1 78.33(19) 3_445 3_545
O2 Ho2 Sb1 138.0(2) 3_455 3_545
Sb2 Ho2 Sb1 73.91(4) 3_545 3_545
Sb2 Ho2 Sb1 108.19(4) 7 3_545
Sb1 Ho2 Sb1 68.27(2) 3 3_545
O3 Ho2 Sb2 79.71(19) . 7_545
O2 Ho2 Sb2 80.01(19) 3_445 7_545
O2 Ho2 Sb2 147.4(2) 3_455 7_545
Sb2 Ho2 Sb2 5.39(12) 3_545 7_545
Sb2 Ho2 Sb2 68.739(15) 7 7_545
Sb1 Ho2 Sb2 110.77(3) 3 7_545
Sb1 Ho2 Sb2 71.23(3) 3_545 7_545
O3 Ho2 Sb2 79.71(19) . 3
O2 Ho2 Sb2 147.4(2) 3_445 3
O2 Ho2 Sb2 80.01(19) 3_455 3
Sb2 Ho2 Sb2 68.739(15) 3_545 3
Sb2 Ho2 Sb2 5.39(12) 7 3
Sb1 Ho2 Sb2 71.23(3) 3 3
Sb1 Ho2 Sb2 110.77(3) 3_545 3
Sb2 Ho2 Sb2 74.13(11) 7_545 3
O3 Ho2 Ho1 36.84(11) . 3_445
O2 Ho2 Ho1 39.6(2) 3_445 3_445
O2 Ho2 Ho1 97.27(19) 3_455 3_445
Sb2 Ho2 Ho1 78.30(3) 3_545 3_445
Sb2 Ho2 Ho1 110.86(3) 7 3_445
Sb1 Ho2 Ho1 173.39(3) 3 3_445
Sb1 Ho2 Ho1 113.336(11) 3_545 3_445
Sb2 Ho2 Ho1 75.59(3) 7_545 3_445
Sb2 Ho2 Ho1 113.12(3) 3 3_445
O3 Ho2 Ho1 36.84(11) . 3_455
O2 Ho2 Ho1 97.27(19) 3_445 3_455
O2 Ho2 Ho1 39.6(2) 3_455 3_455
Sb2 Ho2 Ho1 110.86(3) 3_545 3_455
Sb2 Ho2 Ho1 78.30(3) 7 3_455
Sb1 Ho2 Ho1 113.336(11) 3 3_455
Sb1 Ho2 Ho1 173.39(3) 3_545 3_455
Sb2 Ho2 Ho1 113.12(3) 7_545 3_455
Sb2 Ho2 Ho1 75.59(3) 3 3_455
Ho1 Ho2 Ho1 64.301(13) 3_445 3_455
O3 Ho2 Ho3 95.1(2) . 3_455
O2 Ho2 Ho3 92.53(18) 3_445 3_455
O2 Ho2 Ho3 34.22(19) 3_455 3_455
Sb2 Ho2 Ho3 174.01(2) 3_545 3_455
Sb2 Ho2 Ho3 116.87(6) 7 3_455
Sb1 Ho2 Ho3 77.211(18) 3 3_455
Sb1 Ho2 Ho3 111.01(2) 3_545 3_455
Sb2 Ho2 Ho3 171.71(4) 7_545 3_455
Sb2 Ho2 Ho3 111.51(5) 3 3_455
Ho1 Ho2 Ho3 96.362(18) 3_445 3_455
Ho1 Ho2 Ho3 63.951(15) 3_455 3_455
O2 Ho3 O1 88.1(4) . 3
O2 Ho3 O1 88.1(4) . 3_545
O1 Ho3 O1 117.0(4) 3 3_545
O2 Ho3 O4 168.2(3) . 5_656
O1 Ho3 O4 97.9(4) 3 5_656
O1 Ho3 O4 97.9(4) 3_545 5_656
O2 Ho3 Sb1 84.01(18) . 3_545
O1 Ho3 Sb1 156.05(19) 3 3_545
O1 Ho3 Sb1 85.42(18) 3_545 3_545
O4 Ho3 Sb1 86.43(17) 5_656 3_545
O2 Ho3 Sb1 84.01(18) . 3
O1 Ho3 Sb1 85.42(18) 3 3
O1 Ho3 Sb1 156.05(19) 3_545 3
O4 Ho3 Sb1 86.43(17) 5_656 3
Sb1 Ho3 Sb1 71.29(2) 3_545 3
O2 Ho3 Ho4 127.6(2) . .
O1 Ho3 Ho4 115.7(3) 3 .
O1 Ho3 Ho4 115.7(3) 3_545 .
O4 Ho3 Ho4 40.6(2) 5_656 .
Sb1 Ho3 Ho4 54.924(18) 3_545 .
Sb1 Ho3 Ho4 54.924(18) 3 .
O2 Ho3 Ho2 34.97(9) . 3_545
O1 Ho3 Ho2 106.5(3) 3 3_545
O1 Ho3 Ho2 53.4(3) 3_545 3_545
O4 Ho3 Ho2 148.52(3) 5_656 3_545
Sb1 Ho3 Ho2 79.228(19) 3_545 3_545
Sb1 Ho3 Ho2 114.54(2) 3 3_545
Ho4 Ho3 Ho2 134.149(15) . 3_545
O2 Ho3 Ho2 34.97(9) . 3
O1 Ho3 Ho2 53.4(3) 3 3
O1 Ho3 Ho2 106.5(3) 3_545 3
O4 Ho3 Ho2 148.52(3) 5_656 3
Sb1 Ho3 Ho2 114.54(2) 3_545 3
Sb1 Ho3 Ho2 79.228(19) 3 3
Ho4 Ho3 Ho2 134.149(15) . 3
Ho2 Ho3 Ho2 62.226(14) 3_545 3
O2 Ho3 Ho3 90.000(1) . 1_565
O1 Ho3 Ho3 31.51(18) 3 1_565
O1 Ho3 Ho3 148.49(18) 3_545 1_565
O4 Ho3 Ho3 90.000(1) 5_656 1_565
Sb1 Ho3 Ho3 125.647(10) 3_545 1_565
Sb1 Ho3 Ho3 54.353(10) 3 1_565
Ho4 Ho3 Ho3 90.0 . 1_565
Ho2 Ho3 Ho3 121.113(7) 3_545 1_565
Ho2 Ho3 Ho3 58.887(7) 3 1_565
O2 Ho3 Ho3 90.000(1) . 1_545
O1 Ho3 Ho3 148.49(18) 3 1_545
O1 Ho3 Ho3 31.51(18) 3_545 1_545
O4 Ho3 Ho3 90.000(1) 5_656 1_545
Sb1 Ho3 Ho3 54.353(10) 3_545 1_545
Sb1 Ho3 Ho3 125.647(10) 3 1_545
Ho4 Ho3 Ho3 90.0 . 1_545
Ho2 Ho3 Ho3 58.887(7) 3_545 1_545
Ho2 Ho3 Ho3 121.113(7) 3 1_545
Ho3 Ho3 Ho3 180.00(5) 1_565 1_545
O2 Ho3 Ho1 33.3(2) . .
O1 Ho3 Ho1 105.0(3) 3 .
O1 Ho3 Ho1 105.0(3) 3_545 .
O4 Ho3 Ho1 135.0(2) 5_656 .
Sb1 Ho3 Ho1 58.050(18) 3_545 .
Sb1 Ho3 Ho1 58.050(18) 3 .
Ho4 Ho3 Ho1 94.363(18) . .
Ho2 Ho3 Ho1 56.675(13) 3_545 .
Ho2 Ho3 Ho1 56.675(13) 3 .
Ho3 Ho3 Ho1 90.0 1_565 .
Ho3 Ho3 Ho1 90.0 1_545 .
O1 Ho4 O4 100.3(3) . 3
O1 Ho4 O4 100.3(3) . 3_545
O4 Ho4 O4 115.0(4) 3 3_545
O1 Ho4 O4 175.6(4) . 5_656
O4 Ho4 O4 82.0(2) 3 5_656
O4 Ho4 O4 82.0(2) 3_545 5_656
O1 Ho4 Sb1 91.1(3) . 3_545
O4 Ho4 Sb1 154.63(19) 3 3_545
O4 Ho4 Sb1 84.64(18) 3_545 3_545
O4 Ho4 Sb1 85.31(16) 5_656 3_545
O1 Ho4 Sb1 91.1(3) . 3
O4 Ho4 Sb1 84.64(18) 3 3
O4 Ho4 Sb1 154.63(19) 3_545 3
O4 Ho4 Sb1 85.31(16) 5_656 3
Sb1 Ho4 Sb1 72.46(2) 3_545 3
O1 Ho4 Ho4 143.10(15) . 7_656
O4 Ho4 Ho4 42.9(2) 3 7_656
O4 Ho4 Ho4 100.0(2) 3_545 7_656
O4 Ho4 Ho4 39.07(10) 5_656 7_656
Sb1 Ho4 Ho4 121.25(3) 3_545 7_656
Sb1 Ho4 Ho4 83.356(19) 3 7_656
O1 Ho4 Ho4 143.10(15) . 7_646
O4 Ho4 Ho4 100.0(2) 3 7_646
O4 Ho4 Ho4 42.9(2) 3_545 7_646
O4 Ho4 Ho4 39.07(10) 5_656 7_646
Sb1 Ho4 Ho4 83.356(19) 3_545 7_646
Sb1 Ho4 Ho4 121.25(3) 3 7_646
Ho4 Ho4 Ho4 64.928(19) 7_656 7_646
O1 Ho4 Ho3 137.6(3) . .
O4 Ho4 Ho3 102.1(2) 3 .
O4 Ho4 Ho3 102.1(2) 3_545 .
O4 Ho4 Ho3 37.93(19) 5_656 .
Sb1 Ho4 Ho3 56.097(17) 3_545 .
Sb1 Ho4 Ho3 56.097(17) 3 .
Ho4 Ho4 Ho3 65.835(19) 7_656 .
Ho4 Ho4 Ho3 65.835(19) 7_646 .
O1 Ho4 Ho4 90.000(1) . 1_565
O4 Ho4 Ho4 32.49(18) 3 1_565
O4 Ho4 Ho4 147.51(18) 3_545 1_565
O4 Ho4 Ho4 90.000(1) 5_656 1_565
Sb1 Ho4 Ho4 126.231(11) 3_545 1_565
Sb1 Ho4 Ho4 53.769(11) 3 1_565
Ho4 Ho4 Ho4 57.536(9) 7_656 1_565
Ho4 Ho4 Ho4 122.464(9) 7_646 1_565
Ho3 Ho4 Ho4 90.0 . 1_565
O1 Ho4 Ho4 90.000(1) . 1_545
O4 Ho4 Ho4 147.51(18) 3 1_545
O4 Ho4 Ho4 32.49(18) 3_545 1_545
O4 Ho4 Ho4 90.0 5_656 1_545
Sb1 Ho4 Ho4 53.768(11) 3_545 1_545
Sb1 Ho4 Ho4 126.231(11) 3 1_545
Ho4 Ho4 Ho4 122.464(9) 7_656 1_545
Ho4 Ho4 Ho4 57.536(9) 7_646 1_545
Ho3 Ho4 Ho4 90.0 . 1_545
Ho4 Ho4 Ho4 180.0 1_565 1_545
O1 Ho4 Ho3 29.43(3) . 3_445
O4 Ho4 Ho3 123.1(2) 3 3_445
O4 Ho4 Ho3 73.8(2) 3_545 3_445
O4 Ho4 Ho3 150.653(11) 5_656 3_445
Sb1 Ho4 Ho3 76.259(17) 3_545 3_445
Sb1 Ho4 Ho3 109.94(2) 3 3_445
Ho4 Ho4 Ho3 161.36(3) 7_656 3_445
Ho4 Ho4 Ho3 114.963(12) 7_646 3_445
Ho3 Ho4 Ho3 132.269(18) . 3_445
Ho4 Ho4 Ho3 119.307(6) 1_565 3_445
Ho4 Ho4 Ho3 60.693(6) 1_545 3_445
Ho4 Sb1 Ho4 72.46(2) 3_455 3_445
Ho4 Sb1 Ho3 68.979(17) 3_455 3_455
Ho4 Sb1 Ho3 109.28(3) 3_445 3_455
Ho4 Sb1 Ho3 109.28(3) 3_455 3_445
Ho4 Sb1 Ho3 68.979(17) 3_445 3_445
Ho3 Sb1 Ho3 71.29(2) 3_455 3_445
Ho4 Sb1 Ho2 113.05(3) 3_455 3_445
Ho4 Sb1 Ho2 74.226(18) 3_445 3_445
Ho3 Sb1 Ho2 176.47(3) 3_455 3_445
Ho3 Sb1 Ho2 110.123(10) 3_445 3_445
Ho4 Sb1 Ho2 74.226(18) 3_455 3_455
Ho4 Sb1 Ho2 113.05(3) 3_445 3_455
Ho3 Sb1 Ho2 110.123(10) 3_455 3_455
Ho3 Sb1 Ho2 176.47(3) 3_445 3_455
Ho2 Sb1 Ho2 68.27(2) 3_445 3_455
Ho4 Sb1 Ho1 175.33(2) 3_455 3_445
Ho4 Sb1 Ho1 110.583(10) 3_445 3_445
Ho3 Sb1 Ho1 106.45(3) 3_455 3_445
Ho3 Sb1 Ho1 69.334(18) 3_445 3_445
Ho2 Sb1 Ho1 71.466(17) 3_445 3_445
Ho2 Sb1 Ho1 107.14(3) 3_455 3_445
Ho4 Sb1 Ho1 110.583(10) 3_455 3_455
Ho4 Sb1 Ho1 175.33(2) 3_445 3_455
Ho3 Sb1 Ho1 69.334(18) 3_455 3_455
Ho3 Sb1 Ho1 106.45(3) 3_445 3_455
Ho2 Sb1 Ho1 107.14(3) 3_445 3_455
Ho2 Sb1 Ho1 71.466(17) 3_455 3_455
Ho1 Sb1 Ho1 66.151(19) 3_445 3_455
Ho2 Sb2 Ho2 116.65(13) 3_455 7
Ho2 Sb2 Ho1 75.44(6) 3_455 3_455
Ho2 Sb2 Ho1 73.03(6) 7 3_455
Ho2 Sb2 Ho1 73.03(6) 3_455 7
Ho2 Sb2 Ho1 75.44(6) 7 7
Ho1 Sb2 Ho1 117.70(12) 3_455 7
Ho2 Sb2 Ho2 174.61(12) 3_455 7_545
Ho2 Sb2 Ho2 68.739(15) 7 7_545
Ho1 Sb2 Ho2 107.027(15) 3_455 7_545
Ho1 Sb2 Ho2 109.313(16) 7 7_545
Ho2 Sb2 Ho2 68.739(15) 3_455 3_445
Ho2 Sb2 Ho2 174.61(12) 7 3_445
Ho1 Sb2 Ho2 109.313(16) 3_455 3_445
Ho1 Sb2 Ho2 107.027(15) 7 3_445
Ho2 Sb2 Ho2 105.87(11) 7_545 3_445
Ho2 Sb2 Ho1 107.059(15) 3_455 7_545
Ho2 Sb2 Ho1 109.349(16) 7 7_545
Ho1 Sb2 Ho1 174.65(12) 3_455 7_545
Ho1 Sb2 Ho1 67.651(14) 7 7_545
Ho2 Sb2 Ho1 70.08(6) 7_545 7_545
Ho2 Sb2 Ho1 67.89(6) 3_445 7_545
Ho2 Sb2 Ho1 109.349(16) 3_455 3_445
Ho2 Sb2 Ho1 107.059(15) 7 3_445
Ho1 Sb2 Ho1 67.651(14) 3_455 3_445
Ho1 Sb2 Ho1 174.65(12) 7 3_445
Ho2 Sb2 Ho1 67.89(6) 7_545 3_445
Ho2 Sb2 Ho1 70.08(6) 3_445 3_445
Ho1 Sb2 Ho1 107.00(11) 7_545 3_445
Ho4 O1 Ho3 121.15(18) . 3_445
Ho4 O1 Ho3 121.15(18) . 3_455
Ho3 O1 Ho3 117.0(4) 3_445 3_455
Ho3 O2 Ho2 110.8(2) . 3
Ho3 O2 Ho2 110.8(2) . 3_545
Ho2 O2 Ho2 114.9(4) 3 3_545
Ho3 O2 Ho1 115.4(4) . .
Ho2 O2 Ho1 102.3(2) 3 .
Ho2 O2 Ho1 102.3(2) 3_545 .
Ho1 O3 Ho1 116.9(4) 3_445 3_455
Ho1 O3 Ho2 106.2(2) 3_445 .
Ho1 O3 Ho2 106.2(2) 3_455 .
Ho1 O3 Ho1 104.4(2) 3_445 5_655
Ho1 O3 Ho1 104.4(2) 3_455 5_655
Ho2 O3 Ho1 119.4(4) . 5_655
Ho4 O4 Ho4 115.0(4) 3_445 3_455
Ho4 O4 Ho3 118.7(2) 3_445 5_656
Ho4 O4 Ho3 118.7(2) 3_455 5_656
Ho4 O4 Ho4 98.0(2) 3_445 5_656
Ho4 O4 Ho4 98.0(2) 3_455 5_656
Ho3 O4 Ho4 101.5(3) 5_656 5_656
loop_
_geom_bond_atom_site_label_1
_geom_bond_atom_site_label_2
_geom_bond_distance
_geom_bond_site_symmetry_2
Ho1 O3 2.206(5) 3
Ho1 O3 2.206(5) 3_545
Ho1 O3 2.260(8) 5_655
Ho1 O2 2.306(8) .
Ho1 Sb2 3.269(2) 3_545
Ho1 Sb2 3.269(2) 7
Ho1 Sb1 3.4457(9) 3
Ho1 Sb1 3.4457(9) 3_545
Ho1 Sb2 3.480(2) 7_545
Ho1 Sb2 3.480(2) 3
Ho1 Ho1 3.5292(9) 7_645
Ho1 Ho1 3.5292(9) 7_655
Ho2 O3 2.213(7) .
Ho2 O2 2.231(5) 3_445
Ho2 O2 2.231(5) 3_455
Ho2 Sb2 3.220(2) 3_545
Ho2 Sb2 3.220(2) 7
Ho2 Sb1 3.3510(9) 3
Ho2 Sb1 3.3510(9) 3_545
Ho2 Sb2 3.435(3) 7_545
Ho2 Sb2 3.435(3) 3
Ho2 Ho1 3.5337(6) 3_445
Ho2 Ho1 3.5337(6) 3_455
Ho2 Ho3 3.6392(7) 3_455
Ho3 O2 2.190(8) .
Ho3 O1 2.206(4) 3
Ho3 O1 2.206(4) 3_545
Ho3 O4 2.276(8) 5_656
Ho3 Sb1 3.2266(8) 3_545
Ho3 Sb1 3.2266(8) 3
Ho3 Ho4 3.6289(8) .
Ho3 Ho2 3.6392(7) 3_545
Ho3 Ho2 3.6392(7) 3
Ho3 Ho3 3.7609(2) 1_565
Ho3 Ho3 3.7609(2) 1_545
Ho4 O1 2.205(8) .
Ho4 O4 2.230(4) 3
Ho4 O4 2.230(4) 3_545
Ho4 O4 2.410(8) 5_656
Ho4 Sb1 3.1815(9) 3_545
Ho4 Sb1 3.1815(9) 3
Ho4 Ho4 3.5033(9) 7_656
Ho4 Ho4 3.5033(9) 7_646
Ho4 Ho4 3.7609(2) 1_565
Ho4 Ho4 3.7609(2) 1_545
Ho4 Ho3 3.8416(7) 3_445
Sb1 Ho4 3.1815(9) 3_455
Sb1 Ho4 3.1815(9) 3_445
Sb1 Ho3 3.2266(8) 3_455
Sb1 Ho3 3.2266(8) 3_445
Sb1 Ho2 3.3510(9) 3_445
Sb1 Ho2 3.3510(9) 3_455
Sb1 Ho1 3.4457(9) 3_445
Sb1 Ho1 3.4457(9) 3_455
Sb2 Ho2 3.220(2) 3_455
Sb2 Ho2 3.220(2) 7
Sb2 Ho1 3.269(2) 3_455
Sb2 Ho1 3.269(2) 7
Sb2 Ho2 3.435(3) 7_545
Sb2 Ho2 3.435(3) 3_445
Sb2 Ho1 3.480(2) 7_545
Sb2 Ho1 3.480(2) 3_445
O1 Ho3 2.206(4) 3_445
O1 Ho3 2.206(4) 3_455
O2 Ho2 2.231(5) 3
O2 Ho2 2.231(5) 3_545
O3 Ho1 2.206(5) 3_445
O3 Ho1 2.206(5) 3_455
O3 Ho1 2.260(8) 5_655
O4 Ho4 2.230(4) 3_445
O4 Ho4 2.230(4) 3_455
O4 Ho3 2.276(8) 5_656
O4 Ho4 2.410(8) 5_656
